Università degli Studi di Pisa
Facoltà di Scienze Matematiche Fisiche e Naturali
Scuola di Dottorato Galileo Galilei
Dottorato di Ricerca in Scienze Chimiche
SYNTHESIS AND CHARACTERIZATION OF POLYESTERS FROM
NATURAL SOURCES FOR THE PROTECTION OF STONE
Maria Perla Colombini Piero Frediani
Synthesis and Characterization of Polyesters from Natural Sources
for the Protection of Stone Materials
Presented to the Faculty of “Scienze Matematiche, Fisiche e Naturali” Università degli Studi di Pisa
in Partial Fulfillment of the Requirements for the Degree of
Doctor of Philosophy
Università degli Studi di Pisa
―… I want [young men] see that Nature, if she has given them eyes to see her work …, has also given them the brain for understanding those same works.‖
I would like to thank my advisors, Prof. Piero Frediani and Prof. Maria Perla Colombini, for teaching me the basics of research and for the invaluable help in my work. Thanks to Dr. Luca Rosi and Dr. Marco Frediani for the extensive collaboration and interesting conversations. Thanks to my colleagues and friends Andrea Undri, Guido Giachi, Giulia Giuntoli and Giorgio Petrucci who shared with me this long journey.
Thanks to Dr. Barbara Sacchi, Dr. Emma Cantisani, Dr. Jacopo La Nasa, Dr. Lisa Ghezzi and Dr. Alessio Spepi for the help on various measurements and characterizations.
I would also like to thank all the people at the TEP 243 Nanomaterials Group at the University of Cádiz, Prof. María Jesús Mosquera, Dr. Luís Pinho, Dr. Darío Facio and Dr. Farid Elhaddad for their contribution to this thesis.
Finally I would like to thank my family for the encouragement and support during these years.
Synthesis and Characterization of Polyesters from Natural Sources for
the Protection of Stone Materials
by Andrea Pedna
Stone materials outdoor exposed slowly but inevitably undergo a degradation process, either by natural or artificial causes. The rate of degradation has recently experienced an important acceleration due to natural and anthropic changes in the climatic conditions. It is well known that water plays a central role in the mechanisms of decay (through chemical and physical action), because it is involved in the transport of air pollutants, biodeteriogen growth, transport and crystallization of soluble salts inside the stone and freezing/thaw cycles. In the last decades synthetic polymers have been widely employed for treatment of stone materials as protective coatings, examples being polyacrylates, polysiloxanes and synthetic waxes. However these polymers were chosen among commercial products already available, that often did not meet the requirements for application on artifacts of historical and artistic interest (e.g. minimum alteration, durability and reversibility).
Following the principles of green chemistry, in this work a new class of synthetic polymers derived from polylalctic acid has been developed and tested as protective materials for stone surfaces. By copolymerization of substituted glycolides and lactones, such as lactide, mandelide and salicylide, copolymers with tailor made properties were prepared. Most notably Tg, hydrophobicity and UV barrier properties were improved over conventional PLA. A high and controlled Tg, far from ambient temperature, is
particularly important for a polymer coating, so it never stays in the sticky-rubbery state and is less affected by temperature variations during outdoor exposition. The introduction of perfluorinated chain segments, either by functionalization with perfluoro-alcohols or diols, allowed to improve the hydrorepellency and durability of the coatings. Fluorine containing polymers showed almost no signs of degradation in the accelerated ageing tests, showing excellent stability to photo-oxidative deterioration and negligible color changes.
Another approach to these goals was the synthesis of polylactic acid/silica nanocomposite coatings for the protection of building stones. These organic-inorganic hybrid materials showed improved hydrophobic properties, with water contact angles as high as 137° on stone and glass surfaces, keeping the water barrier properties and durability of fluorinated polylactic acid. A very simple procedure was developed for the synthesis of these materials, by mixing the organic and inorganic components in an organic solution, stirring and directly applying the solution on the surface to be protected. Microscopic analysis (SEM, HAADF-STEM) showed an uniform coating constituted by single particles and larger aggregates covered by the polymer matrix. AFM showed a marked increase of surface roughness, increasing the three-phases contact area between water, air and solid substrate, effectively preventing the penetration of water in the pores of the matrix. Due to the high hysteresis (about 22°) water droplets remained stuck on the surface instead of rolling off, an effect very similar to the natural one occurring on some plants (e.g. rose petals). A reversibility test was carried out by treatment of coated surfaces with organic solvent. The results (AFM, SEM, EDX) indicated that the coating was completely removed, even with the highest silica content, confirming the reversibility of the treatments.
Table of Contents
List of Tables ...x
List of Figures ... xii
List of Schemes ... xvi
Appendix ... xviii
List of Abbreviations ... xix
Chapter 1: Introduction ...24
Polymers for the protection of stone materials ...24
Paraffin wax ...25 Acrylic resins ...27 Silicon resins ...30 Epoxy resins ...33 Polyurethane resins ...35 Fluorinated polymers ...36 Polylactic acid ...42
Functionalization of polylactic acid ...43
Functional monomer route ...44
Alkyl-substituted polyglycolides ...45
Aryl-substituted polyglycolides ...48
Carboxylic acid-substitued polyglycolides ...55
PEG-grafted glycolides ...60
Alkenyl- and alkynyl-substitued polyglycolides ...62
Polylactic acid nanocomposites ...66
Chapter 2: Synthesis of PLA copolymers with perfluorinated chain segments...73
Results and discussion ...76
Monomers synthesis...76 Polymers synthesis ...78 LD/MD copolymerization ...81 PMGLY polymerization ...88 SALD polymerization ...94 FLK block copolymers ...100 Conclusions ...105 Experimental Section ...106
Chapter 3: Evaluation of polymers as protective coatings for stone materials ...112
Results and discussion ...114
Selection of polymers ...114
Application of polymers as stone coatings ...118
Evaluation as protective coatings ...121
Chromatic variations ...121
Contact angle ...123
Capillary water absorption ...125
Water Vapor Permeability ...127
Artificial ageing ...128
Molecular weight determination ...130
Thermal properties ...135
FT-IR spectra ...135
Chromatic variations ...146
Py-GC/MS analysis ...152
Experimental section ...155
Chapter 4: PLA/SiO2 nanocomposites as coatings for stone materials ...158
Results and discussion ...161
Synthesis and chatacterization ...161
Textural properties ...162
Application to glass surfaces ...169
Contact angle ...169
SEM and AFM ...173
Application to stone surfaces ...176
Contact angle ...177
SEM and AFM ...178
Specific tests for conservation materials...183
Reversibility test ...183 Conclusions ...186 Experimental Section ...187 Chapter 5: Conclusions ...191 Appendix ...194 References ...214
List of Tables
Table 1. Reaction conditions and product characterization of LD/MD
copolymerizations. ... 83 Table 2. DSC analysis of LD/MD copolymers. ... 84 Table 3. TGA analysis of LD/MD copolymers. ... 86 Table 4. Reaction conditions and product characterization of PMGLY
polymerizations. ... 89 Table 5. Reaction conditions and product characterization of SALD
polymerizations. ... 95 Table 6. Reaction conditions and product characterization of FLK block
copolymerizations. ... 100 Table 7. Products applied as stone coatings with selected characteristics. ... 115 Table 8. Protective efficacy and vapor diffusivity of the treatments. ... 127 Table 9. Physicochemical characteristics of poly(LD-co-MD) sample unaged and
at different steps of the artificial ageing process. ... 139 Table 10. Physicochemical characteristics of poly(PMGLY) and poly(PMGLY)-F
samples unaged and at different steps of the artificial ageing process. ... 140 Table 11. Physicochemical characteristics of poly(SALD) and poly(SALD)-F
samples unaged and at different steps of the artificial ageing process. ... 142 Table 12. Physicochemical characteristics of PMGLY-FLK-PMGLY and
SALD-FLK-SALD samples unaged and at different steps of the artificial
ageing process. ... 144 Table 13. Protective efficacies (E%) of treatments after 1000 h of artificial
Table 14. Formulation and textural parameters of the nanocomposites under
study. ... 162 Table 15. Contact angles of water droplets on glass surfaces coated by
dip-coating. Errors are reported as standard deviations. ... 172 Table 16. Contact angles of water droplets on glass surfaces coated by solution
casting. Errors are reported as standard deviations. ... 172 Table 17. Contact angles of water droplets on marble surfaces coated by solution
casting. Errors are reported as standard deviations. ... 178 Table 18. Protective efficacy (E%), water vapor permeability and color change
List of Figures
Figure 1. Structures of acrylic (a) and methacrylic (b) polymers. ... 27
Figure 2. Some examples of fluorinated acrylates and methacrylates. ... 41
Figure 3. Alkyl-substituted polyglycolides with their respective Tg. ... 48
Figure 4. Aryl-substitued polyglycolides with their respective Tg. ... 50
Figure 5. PLA-bionanocomposites processing techniques. ... 70
Figure 6. Structure of poly(mandelide) and poly(salicylide). ... 74
Figure 7. 1H-NMR spectrum of LA/MD copolymer (run 4, Table 1). Monomers insertion was determined from the relative intensity of signals b and c (LD = 85.9%, MD = 14.1%). ... 81
Figure 8. DSC scans of poly(lactide) (PLA) and poly(mandelide) (PMD) samples. PMD was an amorphous material and showed an increased Tg value. ... 85
Figure 9. TGA thermograms of LD/MD copolymers at different compositions. ... 87
Figure 10. UV-VIS absorption spectra of 1 g/L solutions of LD/MD copolymers at different composition. ... 87
Figure 11. 1H-NMR (top) and 13C-NMR (bottom) spectra of poly(PMGLY) (run 8, Table 4). ... 90
Figure 12. 1H-NMR (top) and 19F-NMR (bottom) spectra of poly(PMGLY) functionalized with PFoct (run 10, Table 4). ... 91
Figure 13. 1H-NMR (top) and 13C-NMR (bottom) spectra of poly(SALD) (run 13, Table 5). ... 98
Figure 14. 1H-NMR (top) and 19F-NMR (bottom) spectra of poly(SALD) functionalized with PFoct (run 17, Table 5). ... 99
Figure 15. 13C-NMR spectra of PMGLY-FLK-PMGLY (top) and
SALD-FLK-SALD (bottom). ... 103 Figure 16. 19F-NMR spectra of PMGLY-FLK-PMGLY (top) and
SALD-FLK-SALD (bottom). ... 104 Figure 17. FT-IR spectra of polymers applied as stone coatings. ... 120 Figure 18. Chromatic variations of marble samples after treatment with the
products (error bars representing standard deviations). ... 122 Figure 19. Static contact angle on marble surfaces treated with the products (error
bars representing standard deviations). ... 125 Figure 20. Weight loss of the samples during artificial ageing. ... 129 Figure 21. GPC chromatograms of poly(PMGLY) (top) and poly(PMGLY)-F
polymers (bottom) unaged and at different steps of the artificial ageing process. ... 132 Figure 22. GPC chromatograms of poly(SALD) (top) and poly(SALD)-F
(bottom) polymers unaged and at different steps of the artificial ageing process. ... 133 Figure 23. GPC chromatograms of PMGLY-FLK-PMGLY (top) and
SALD-FLK-SALD (bottom) polymers unaged and at different steps of the
artificial ageing process. ... 134 Figure 24. FT-IR spectra of poly(LD-co-MD) sample unaged and after 1000
hours of artificial ageing. ... 139 Figure 25. FT-IR spectra of poly(PMGLY) (top) and poly(PMGLY)-F (bottom)
samples unaged and at different steps of the artificial ageing process. ... 141 Figure 26. FT-IR spectra of poly(SALD) (top) and poly(SALD)-F (bottom)
Figure 27. FT-IR spectra of PMGLY-FLK-PMGLY (top) and SALD-FLK-SALD (bottom) samples unaged and at different steps of the artificial ageing
process. ... 145 Figure 28. Chromatic variations of marble samples after treatment with
poly(PMGLY) (top) and poly(PMGLY)-F (bottom) coatings unaged and at different ageing times (error bars representing standard
deviations). ... 149 Figure 29. Chromatic variations of marble samples after treatment with
poly(SALD) (top) and poly(SALD-F) (bottom) coatings unaged and at
different ageing times (error bars representing standard deviations). ... 150 Figure 30. Chromatic variations of marble samples after treatment with
PMGLY-FLK-PMGLY (top) and SALD-FLK-SALD (bottom) coatings unaged and at different ageing times (error bars representing standard
deviations). ... 151 Figure 31. Typical pyrogram of poly(LD-co-MD) copolymer and assignment of
main peaks... 153 Figure 32. Spectral irradiance of the Xenon lamp with the outdoor UV filter used
in the artificial ageing tests. ... 157 Figure 33. Nanocomposite synthesis procedure. ... 161 Figure 34. Nitrogen isotherms (top) and BJH pore size distribution (bottom) for
the nanocomposites under study. ... 164 Figure 35. HAADF-STEM images of PLDA-FLK-PLDA, P-S20 and P-S80 and
TEM image of AE-OX50 commercial SiO2 nanoparticles. ... 166 Figure 36. EDX elemental analysis of product P-S80. ... 167
Figure 37. FT-IR spectra of PLDA-FLK-PLDA/SiO2 nanocomposites with
different SiO2 content... 168 Figure 38. Static and dynamic contact angles for glass surfaces treated with
nanocomposites by dip-coating (top) and solution casting (bottom)
techniques (bars representing standard deviations). ... 171 Figure 39. SEM and AFM 2D images of product films casted on glass support. ... 174 Figure 40. AFM 3D images and roughness size distribution for products under
study casted on glass support. ... 175 Figure 41. FT-IR spectra of PLDA-FLK-PLDA/SiO2 nanocomposites with
different SiO2 content applied on the surface of marble. ... 179 Figure 42. Static and dynamic contact angles for marble surfaces treated with
PLDA-FLK-PLDA/SiO2 with different SiO2 content (bars
representing standard deviations). ... 180 Figure 43. SEM and AFM 2D images of untreated and coated marble samples. ... 181 Figure 44. AFM 3D images and roughness size distribution for untreated marble
and products under study casted on marble support. ... 182 Figure 45. SEM micrographs of marble surfaces employed in the reversibility
test. AFM and EDX measurements before (left) and after (right)
List of Schemes
Scheme 1. Copolymerization of ethylene with UDO (a) and MOD (b). ... 26 Scheme 2. Basic hydrolysis of inorganic silicates... 30 Scheme 3. Condensation polymerization of a siloxane monomer. ... 30 Scheme 4. Condensation between epichloridrin and bis-phenol-A (a) and cross-linking of the epoxy prepolymer to obtain the epoxy resin (b). ... 34 Scheme 5. Synthesis of a polyurethane resin. ... 35 Scheme 6. Synthesis of some important families of perfluoropolyethers with commercial
names. ... 38 Scheme 7. Mechanism of the ROP process of lactide. ... 43 Scheme 8. Different routes to PLA functionalization (FG = functional group). ... 44 Scheme 9. General scheme of the synthesis of symmetric and asymmetric glycolides. ... 45 Scheme 10. Comparison between copolymerization of symmetric glycolides and
homopolymerization of asymmetric glycolides. ... 47 Scheme 11. Synthesis, polymerization and deprotection of 3-BMG. ... 51 Scheme 12. Synthesis, polymerization, and deprotection of Ser-GLY and OBn-L-Ser-LD. ... 53 Scheme 13. Synthesis, polymerization, and partial deprotection of DiPAGYL and
DiPALAC. ... 54 Scheme 14. Synthesis, polymerization, and deprotection of
3(S)-[(benzyloxycarbonyl)methyl]-1,4-dioxane-2,5-dione. ... 55 Scheme 15. Synthesis of malide dibenzyl ester from L-malic acid (L-MA) or L-aspartic
acid (L-Asp), polymerization, and deprotection. ... 56 Scheme 16. Synthesis, polymerization, and deprotection of OBn-L-Glu-LD. ... 57
Scheme 17. Synthesis, polymerization, and deprotection of Cbz-L-Lys-LD... 58
Scheme 18. Synthesis, polymerization and deprotection of 3-[Nε -(carbonylbenzoxy)-L-lysyl]-6-L-methyl-morpholine-2,5-dione. ... 60
Scheme 19. Synthesis and polymerization of a PEG-grafted glycolide. ... 62
Scheme 20. Synthesis and polymerization of diallylglycolide. ... 64
Scheme 21. Synthesis, polymerization and post-functionalization of allylglycolide. ... 65
Scheme 22. Synthesis and polymerization of propargyl glycolide. ... 66
Scheme 23. Synthesis of functionalized ROP monomers mandelide (MD), salicylide (SA), phenylmethylglycolide (PMGLY) and salicyllactide (SALD). ... 78
Scheme 24. Polymerization of ROP monomers to obtain lactic acid/mandelic acid and lactic acid/salicylic acid copolymers. ... 79
Scheme 25. Propagation pathways in the polymerization of an AB monomer . ... 92
Scheme 26. Different pathways in the SALD polymerization catalyzed by DMAP . 97 Scheme 27. Synthesis of FLK block copolymers PLDA-FLK-PLDA (a), PMGLY-FLK-PMGLY (b), SALD-FLK-SALD (c). ... 101
Scheme 28. Main bond scissions of poly(lactic acid/mandelic acid) by direct photolysis during UV ageing. ... 137
Scheme 29. Main degradation reactions involved in the thermal ageing of poly(LD-co-MD) in the presence of hexamethyldisiloxane (HMDS). ... 153
Appendix 1. 1H-NMR spectra of 3,6-diphenyl-1,4-dioxane-2,5-dione (MD). ... 195
Appendix 2. 13C-NMR spectra of 3,6-diphenyl-1,4-dioxane-2,5-dione (MD). ... 196
Appendix 3. 1H-NMR of dibenzo-1,5-dioxocin-6,12-dione (SA). ... 197
Appendix 4. 1H-NMR of (3S)-6-methyl-3-phenyl-1,4-dioxan-2,5-dione (PMGLY). .... 198
Appendix 5. 13C-NMR of (3S)-6-methyl-3-phenyl-1,4-dioxan-2,5-dione (PMGLY). ... 199
Appendix 6. 1H-NMR of 2-((2-bromopropanoyl)oxy)-2-phenylacetic acid. ... 200
Appendix 7. 1H-NMR of 1,4-benzodioxepin-3-methyl-2,5-dione (SALD)... 201
Appendix 8. 13C-NMR of 1,4-benzodioxepin-3-methyl-2,5-dione (SALD). ... 202
Appendix 9. 1H-NMR of 2-((2-bromopropanoyl)oxy)benzoic acid. ... 203
Appendix 10. 1H-NMR of 2-hydroxy-2-phenylacetic acid (mandelic acid). ... 204
Appendix 11. 1H-NMR of 2-hydroxybenzoic acid (salicylic acid). ... 205
Appendix 12. 1H-NMR of 2-bromopropionil bromide. ... 206
Appendix 13. 1H-NMR of 3,3,4,4,5,5,6,6,7,7,8,8,8-tridecafluoro-1-octanol (PFoct). ... 207
Appendix 14. 13C-NMR of 3,3,4,4,5,5,6,6,7,7,8,8,8-tridecafluoro-1-octanol (PFoct). .. 208
Appendix 15. 19F-NMR of 3,3,4,4,5,5,6,6,7,7,8,8,8-tridecafluoro-1-octanol (PFoct). ... 209
Appendix 16. 19F-NMR of Fluorolink D10-H (FLK). ... 210
Appendix 17. 1H-NMR of poly(PMGLY) after 500 h of artificial ageing. ... 211
Appendix 18. 1H-NMR of poly(PMGLY) after 750 h of artificial ageing. ... 212
List of Abbreviations
3-BGM 3-benzyloxymethyl-1,4-dioxane-2,5-dione 3-HGM 3-hydroxymethyl-1,4-dioxane-2,5-dione
AFM atomic force microscopy
ATR attenuated total reflectance
ATRP atom transfer radical polymerization
BA butyl acrylate
BBA 4-tert-butylbenzyl alcohol
BET Brunauer–Emmett–Teller BJH Barret-Joyner-Halenda CA contact angle CFC chlorofluorocarbon CL ε-caprolactone CNT carbon nanotube Cp heat capacity d doublet δ chemical shift DCC N,N'-dicyclohexylcarbodiimide DGEBA diglycidyl ether of bis-phenol-A DIEA N,N-diisopropylethylamine DMAP 4-(dimethylamino)-pyridine
DMSO dimethyl sulfoxide
DMSO-d6 deuterated dimethyl sulfoxide
DiPALAC 3-methyl-6-(1,2,3,4-tetraoxobutyl-diisopropylidene)-dioxane-2,5-dione DSC differential scanning calorimetry
E% protective efficacy
EDX energy dispersive spectroscopy
EMA ethyl methacrylate
EPMgMA maleic anhydride-grafted ethylene propylene rubber f-MWCNT functionalized multiwalled carbon nanotube
FG functional group
FLK Fluorolink D10-H
FM functional monomer
FT-IR fourier transform-infrared
GC gas chromatography
GPC gel permeation chromatography
HAADF-STEM high-angle annular dark-field scanning transmission electron microscopy Hc enthalpy of crystallization Hm enthalpy of fusion HMDS hexamethyldisiloxane Hz Hertz J coupling constant kD kiloDalton
L-LA L-aspartic acid
L-MA L-malic acid
MA methyl acrylate
mCPBA meta-chloroperoxybenzoic acid
MMA methyl methacrylate
Mn number average molecular weight
MOD ethylene/7-methyl-1,6-octadiene mPEG poly(methoxy-ethylene glycol)
MS mass spectrometry
Mw weight average molecular weight
NMO N-methylmorpholine N-oxide
NMR nuclear magnetic resonance o-PCL oligo(ε-caprolactone)
OMMT organically modified montmorillonite PBMA poly(butyl methacrylate
PE2FA poly(ethyl 2-fluoroacrylate)
PDI polydispersity index
PEG poly(ethylene glycol)
PET poly(ethylene terephthalate)
PFoct 3,3,4,4,5,5,6,6,7,7,8,8,8-tridecafluoro-1-octanol, perfluoro-octanol PFPE perfluoropolyethers
PLA poly(lactide), polylactic acid
PLLA-FLK-PLLA L-lactide/Fluorolink D10-H block copolymer PLDA-FLK-PLDA rac-lactide/Fluorolink D10-H block copolymer
PMGLY-FLK-PMGLY phenylmethylglycolide/Fluorolink D10-H block copolymer
PMMA poly(methyl methacrylate)
POSS oligomeric silsesquioxane
ppm part per milion
pTSA para-toluensulphonic acid
Py-GC/MS pyrolysis–gas chromatography–mass spectrometry
rac-LD racemic lactide
rac-MD racemic mandelide
ROP ring opening polymerization
SALD-FLK-SALD salicyl lactide/Fluorolink D10-H block copolymer SEC size exclusion chromatography
SEM scanning electron microscopy
SnOct2 Sn(II) Octoate, Sn(II)-2-ethylesanoate
Tc crystallization temperature
Td decomposition temperature
TEM transmission electron microscopy TEOS tetraethyl orthosilicate
Tg glass transition temperature
TGA thermogravimetric analysis
THF tetrahydrofuran Tm melting temperature TPS thermoplastic starch UDO 10-undecen-1-ol UV ultraviolet UV-vis ultraviolet-visible Xc degree of crystallinity
Chapter 1: Introduction
POLYMERS FOR THE PROTECTION OF STONE MATERIALS
All stone materials exposed to an outdoor environment inevitably go through a deterioration process, either by artificial or natural causes. Water plays a central role in the deterioration, because it is involved in the transport of air pollutants (e.g. CO2, SO2, NOx) inside stones; moreover it improves biodeteriogen growth and causes mechanical stress as a consequence of the crystallization of soluble salts transported by water inside the stone and by freezing/thaw cycles .
A polymer employed for the protection of stone material (stone protective) is a substance that is applied on the surface avoid degradation processes. The protective should form a coating that acts as a barrier against water penetration (either rain or condensation water) and atmospheric pollutants, however keeping the water vapor permeability of the stone . The main properties of a protective material are: (1) hydrorepellency, that depends mainly on the chemical composition and structure of the product, and the distribution of the coating on the surface; (2) adhesion, that is the ability to stick to the surface and resist to mechanical stress due to atmospheric agents and temperature variations; (3) resistance to degradation, the material should be inert, that is it should have thermal and photo-oxidative stability, and does not release harmful substances during its degradation; (4) reversibility, the treatment should be completely reversible allowing to regain the starting conditions of the surface at any time, to allow treatment with another product or removal at the end of its service life. In addition the principle of “minimum alteration” should be followed, that involves mainly the optical properties of the treated artifact (i.e. color changes and transparency of the coating). Today there is no commercial product available that simultaneously meets all the
aforementioned requirements. Furthermore the performance of a product often vary with the specific application (nature of the substrate, application method, exposure conditions, etc.). In the following paragraphs the main products employed for the conservation of stone materials are descripted in details, with a special attention to the aspects regarding the conservation of Cultural Heritage.
Aliphatic wax hydrocarbons are obtained as a heavy fraction in the refining of oil or by polymerization of ethylene. They are mainly constituted by linear aliphatic hydrocarbons having relatively low molecular weight. They have a high resistance to ageing and optical properties close to those of natural resins. They are mainly employed as varnishes for panel or canvas paintings. Due to the low polarity, when applied on stone materials, they easily diffuse inside the stones .
Synthetic products with a hydrocarbon structure are widely employed in the field of conservation, such as microcrystalline waxes (e.g. Cosmolloid 80) and aliphatic varnishes (e.g. Regalrez 1094). One of the main problems when these products are employed for stone conservation is the rather low ability to interact with stone surface due to their apolar structure. This leads to a migration of the product inside the stone and a loss of protection efficacy when exposed to an open air. Recently an attempt to solve these problems was made with the synthesis of polar functionalized polyolefins specifically designed for stone protection . Ethylene/10-undecen-1-ol (ethylene/UDO) and ethylene/7-methyl-1,6-octadiene (ethylene/MOD) copolymers, containing polar groups, were synthetized by Ziegler-Natta catalysis (Scheme 1). Ethylene/MOD copolymer was further functionalized by hydroesterification and hydrogenation. The final
products were composed by linear polyethylene chains with branching moieties containing hydroxy and ester groups, more compatible with inorganic substrates. The performance of these products was tested on selected marble and Lecce stone specimens with very different porosity and pore size distribution.
Ethylene/MOD copolymer was obtained as an amorphous material and showed interesting film forming properties and very high water repellency. However a loss of protection efficacy was observed when exposed to artificial ageing, caused by photo-degradation and oxidation reactions.
Ethylene/UDO had a more crystalline character and its solubility was strongly affected by molecular weight distribution. The protective performance was higher when applied on the high porosity Lecce stone rather than on low porosity marble substrate. The product showed high stability to photo-oxidation and kept the protection efficacy even after 1000 h of exposure to UV radiations.
Acrylic polymers are widely used for the formulation of protective products, due to their good adhesion, transparency and film forming properties. Acrylic resins are also used as consolidant and adhesive products. They are thermoplastic materials, obtained from homo- or copolymerization of esters of acrylic and methacrylic acid (Figure 1). Their molecular weights are in the range 30-100 kDa: the characteristics of an acrylic product can be quite different, according to the monomer employed (acid moiety: acrylic or methacrylic; ester moiety: methyl, ethyl, propyl, butyl, etc.) and the molecular weight.
Figure 1. Structures of acrylic (a) and methacrylic (b) polymers.
Polymer rigidity and “rubbery grade” change according to the acid moiety of the starting monomers (methacrylic are more hard and rigid than acrylic esters) and the chain length of the ester group. As an example, poly(methyl methacrylate) (PMMA) is hard and fragile, while poly(butyl methacrylate) (PBMA) is an oil at room temperature. Most of acrylic resins are soluble in common organic solvents, like ketones, esters, aromatic hydrocarbons and chlorinated solvents, and have good adhesive properties. Their glass transition temperature (Tg) and melting temperature (Tm) can be very different, so copolymers with wide range of rigidness and hardness can be obtained. These properties
may be modulated selecting different ratios among monomers and modifying the molecular weight of the polymer in order to obtain the desired Tg and Tm.
Paraloid B-72 (a polymer among ethyl methacrylate (EMA) and methyl acrylate (MA) (70/30) with low amount of butyl acrylate (BA)) is a commercial product, which is extensively used since 1970 as a consolidant and protective agent. It offers quite good hydrorepellency, high transparency, hardness, partial reversibility and moderate stability . Other commercial products, such as Primal AC33 (a copolymer between methyl methacrylate and ethyl acrylate (MMA and EA)), Paraloid B67 (poly(isobutyl methacrylate)), Elvacite 2010 (poly(methyl methacrylate) (PMMA)) were extensively used in the past decades .
Acrylic resins have some limits, as the other categories of protective products. One of the most common problems noticed with these polymers is a low penetration of the product inside the stone material: even in the better conditions of application (a good solvent and a low viscosity of the solution), a penetration deeper than 1 cm is very hard to be reached. Another limit observed with acrylic resins is that they act as water repellents only for a limited period of time. In order to obtain a long-lasting effect, acrylic polymers are often applied in mixture with silicon resins, or as a fluorinated acrylic polymer.
The acrylic resins in the course of the ageing lose hydrophobicity, solubility and turn yellow, as a function of their exposure to atmospheric agents. In order to obtain protectives having a high thermal and photo-stability, a great variety of acrylic homopolymers and acrylic/methacrylic copolymers has been extensively investigated [5-9]. Acrylic polymers give rise to crosslinking, while methacrylic ones are subjected to depolymerization. The C-H bond of the tertiary carbon in PMA can be easily homolitically broken generating two radicals; these radicals can react with other radicals, giving a new C-C bond, that is a cross-linking between two different molecules. The
result of this reaction is an increase of the molecular weight of the polymer with loss of its solubility and flexibility. These changes may cause fractures on the film protecting the surface and lack of reversibility.
In the case of PMMA there are no tertiary carbon atoms in the molecule, but the C-CH3 bond of side chains may be broken, generating a C=C double bond. This process may be followed by depolymerization, decreasing the molecular weight and a partial loss of the polymer from the protected surface. Alternatively, if conjugated double bonds are formed, they may give origin to chromophoric groups that are responsible for film yellowing. If the polymers are employed as protective coatings for the conservation of monuments or ancient buildings, the limited environmental stability of acrylic polymers makes them inadequate, in the long term, to fulfill the requirements of water repellence, water vapor permeability, reversibility and negligible influence on the color of the substrates.
To overcome the aforementioned limitations, blendings with inorganic oxides have been proposed. The blending with anatase (TiO2) nanoparticles was performed [10, 11], in consideration of its photocatalytic activity in the oxidation of organic contaminants and bacteria . However some problems arose because the nanoparticles are highly hydrophilic while polyacrylates are hydrophobic and the polymer may be oxidized by the catalytic activity of anatase. Also a blending of Paraloid-B72 and nanoparticles of calcium hydroxide [Ca(OH)2] has been suggested for the protection of stones or plasters .
Silicon resins are wide class of products that are used in the conservation field since the sixties [14-16]. These compounds contain many Si-O bonds, possessing a high stability (higher than C-C, C-O and Si-Si bonds). Inorganic silicates, such as Na2SiO3 and K2SiO3, where firstly used as stone consolidants, but some reaction products may be dangerous to the stone itself (Scheme 2).
Scheme 2. Basic hydrolysis of inorganic silicates.
In the case of organic silicon compounds (siloxanes), silicon may form two bonds with oxygen atoms, while remains the possibility to form two other bonds with different groups (Scheme 3). The groups linked to silicon deeply affect the properties (and hence the performances) of the siloxanes. As an example, large substituents lead to rigid chains (high Tg), while silicon bonded to small groups show a low Tg. The length of the chain is another parameter affecting the properties of the resins. As a general rule, siloxanes with less than 10 silicon groups are liquid at room temperature, otherwise they are waxy and stiff.
In all silicon monomers or prepolymers, the Si-O-C moieties undergo an easy hydrolysis when exposed to water, then the formed Si-OH groups covalently bind to superficial O-H groups present on the stone and polymerize, giving rise to linear or branched structures, depending on the number of the O-H groups present on a silicon atom. The rate of hydrolysis and subsequent polymerization of siloxane is strongly affected by the relative humidity of the environment and hence from atmospheric conditions.
The alkyl-alkoxysilanes have general formula RnSi(OR’)m (n = 1, 2, m = 2, 3), the silicon atom is linked to alkyl and alkoxy groups. They are mainly used as monomers, in order to obtain an “in situ” polymerization. The alkyl-alkoxysilanes monomers show a low molecular weight and they can deeply penetrate even in materials having a low porosity. On the other hand monomers are quite volatile, so they can be removed by evaporation or washed away before polymerization. The rate of polymerization depends on the humidity present in the stone and in the atmosphere, so the process is not easily reproducible. Furthermore the molecular weight distribution is large and difficult to reproduce.
Alkyl-alkoxysilanes prepolymers can also be employed: Si-O-C bonds may hydrolyze when the product is penetrated inside the stone and gives further polymerization. Their volatility is low, avoiding the loss of product by evaporation or washing before the complete polymerization. Both monomers and oligomers have good hydrorepellency, due to the film formation properties and water insolubility. Furthermore, they have good interaction with substrate. The polymers formed are not reversible because they are not soluble in common solvents, so they are very hard to remove.
In polysiloxanes, silicon forms two bonds with two alkyl (or aryl) groups. These groups may be the same or different. The polysiloxanes employed have high molecular weights and their structures can be linear, branched or cross-linked, containing alkyl and/or aryl groups giving flexibility and hydrophobicity. They keep the initial solubility when applied, but their penetration in a porous substrate is low, as usually happens for all high molecular weight polymers. These products seem to have a good protective efficacy towards pollutant agents like SO2 and NOx. Moreover, they have a good hydrorepellency, so they demonstrate a good protection even to freeze/thaw phenomena. Regarding the permeability to water vapor and the stability to UV radiation, the results reported in literature are controversial [17, 18].
Silanols containing at least two alcoholic groups linked to silicon may be employed and, after the application of the product, hydroxyl groups react with the same groups of other molecules, giving rise to a Si-O bond. The other bonds of silicon may be engaged by alkyl or aryl groups.
Lastly, the alkoxysilanes are considered on the borderline between inorganic and organic products, because silicon is linked to four alkoxy groups. The most widespread alkoxysilane is tetraethyl orthosilicate (TEOS), that is a low molecular weight product having low density. The reactions involved are close to those of alkyl-alkoxysilanes, with hydrolysis and condensation that leads to tridimensional silicate polymer. The absence of alkyl groups in the structure does not give hydrorepellent properties, but it has good performances as consolidant.
In recent years a new class of composite silicon material has been developed. It is based on organic polymers and inorganic layered reinforcement, consisting of organo-modified silicates whose layers have a thickness of few nanometers [19, 20]. These systems show a large interfacial area in the range between nanosheets and polymer, with
better properties if compared to unmodified resins. In particular they exhibit higher chemical, thermal and mechanical resistance and reduced gas and vapor permeability, without spoiling the optical properties of the polymeric matrix.
The addition of silica nanoparticles substantially enhances the protective efficiency of silicon compounds and the treated stone surface is super-hydrophobic and may be self-cleaning [21, 22]. In another application the addition of nanolime, that is nanoparticles of calcium hydroxide (nanorestore), improved the consolidating performances of the blending .
Polysiloxane and fluorine containing siloxane polymers have been developed and used for the protection of building materials . The inclusion of fluorinated molecules reduced the already low surface energy of alkyl-siloxanes. Thanks to the greater mobility of the siloxane chain, fluorocarbon groups could be aligned more effectively on the surface of the polymer. In addition the water and oil repellence was increased by the presence of fluorine, enhancing also the chemical, thermal and photo-chemical stability.
Epoxy resins are low molecular weight linear polymers obtained from monomers or short chain polymers containing epoxy groups at both ends of the chain . One of the most common epoxy pre-polymer is obtained from the reaction between epichlorohydrin and bis-phenol-A. Similar prepolymer can be obtained by substitution of one or both chemicals employed. The further reaction of the prepolymer with a cross-linking agent, usually a diamine, gives the epoxy resin (Scheme 4).
Scheme 4. Condensation between epichloridrin and bis-phenol-A (a) and cross-linking of the epoxy prepolymer to obtain the epoxy resin (b).
One of the commercial epoxy resins is obtained from the diglycidyl ether of bis-phenol-A (DGEBA). It is a viscous oligomer that can be applied together with a catalyst and a cross-linking agent to form the final polymer. Epoxy resins are highly resistant to acids, bases and organic solvents but show serious problems of color stability: usually these resins become yellow even when stored in the absence of light.
Epoxy resins have been widely used and tested as adhesives for sticking glass object that will be stored in the museum environment. Due to the high strength and gap-filling ability, epoxy resins were used for the consolidation and restoration of stone, even if they show a quite important absorption of SO2. On the contrary, they are not utilized as protective materials, since they do not contain hydrophobic groups.
Polyurethanes are synthesized by reacting a monomer containing at least two isocyanate functional groups with a molecule containing at least two hydroxyl groups  (Scheme 5). They are largely used in a number of applications, including daily home furniture, cars and thermal isolation. In the conservation field, polyurethanes are mainly employed to seal surfaces of different materials such as wood, metal, and paintings or to protect them from rot, corrosion, or fading. As an example, Xylamon LX Hardening N (Desowag) has been extensively used since 1950s for the consolidation of fragile wood. Commercial polyurethanes have been used for the conservation of leather, both as adhesives and consolidants [25, 26]. Rigid polyurethane foams using an appropriate isolating varnish have been used for temporary facing supports in the course of a painting restoration . As adhesives, polyurethanes resist to moisture and heat, so their use is ideal in the case of objects exposed, particularly to sun and salted waters.
Scheme 5. Synthesis of a polyurethane resin.
Nevertheless, polyurethane resins are not extensively used in conservation, because all isocyanate monomers are highly toxic. Furthermore, polyurethane polymers are sensitive to thermal and photo-oxidative degradation . Especially polyurethane foams can turn yellow and disintegrate, so it is widely used in the lifting and temporary
support of archaeological objects, but when a long life is required, polyurethane foams are substituted by polyether foams.
Polyurethane polymeric structures with fluorinated segments in their chains provide a higher stone protection than perfluoropolyetheres alone. C-F bond makes the polymer hydrorepellent and chemically stable and, on the other side, the polarity of urethane bond may help to link the film on the stone substrate, reducing stone decay. Another advantage of these products is the possibility to perform the synthesis using a water emulsion.
In order to improve the properties of polymers used in conservation of stone materials, since the end of seventies, Piacenti’s group proposed the use of perfluoropolyethers . These polymers were promising protectives from different points of view: they provided excellent hydrophobicity, high resistance to UV radiation, inertia towards the substrate and most of the pollutants present in the atmosphere. Fluorinated organic molecules are indeed chemically and thermally very stable, due to the high energy of the C-F bond and to the deactivation effect induced by the electronegative fluorine atoms towards the C-C bonds.
Fluorinated elastomers have a good capacity of adhesion and cohesion, and they are used mainly as adhesives and binders in fillers, but some of them also have protective properties (an example is the commercial product known as NH). However, elastomers have large molecular dimensions, so they are not able to deeply penetrate inside stone materials, and they show good performances mainly on lithotypes having a high porosity.
Perfluoropolyethers on the contrary have medium or low molecular weights, usually between 5000 and 7000 Da, and a good penetration capacity. They are obtained from the photo-oxidative-polymerization of hexafluoropropylene or tetrafluoroethylene and they were tested and then suggested as water repellents in the field of stone conservation of monumental buildings (Scheme 6) [29-33]. In consideration of their water- and dirt-repellent properties, fluorinated products have been used primarily to develop waterproof coatings, but some researches has been also reported on their anti-graffiti properties . Perfluoropolyethers are extremely stable, colourless, permeable to oxygen, insoluble in water and most of the organic solvents. Moreover, they are liquid and therefore easily applicable on a solid surface. Furthermore they are not toxic, have a low superficial tension and a refractive index very close to that of water. Akeogard PF and Fomblin Y MET were commercial products largely diffused in the past years.
Unfortunately the good preliminary results were followed by some negative features, particularly color changes and reduction of protective efficacy in relatively short times when applied on some lithotypes. Regarding color changes, it was noticed that this behavior is not due to a degradation of the product, but to the inclusion of dust particulate on the surface, leading to a darkening of the surface itself, especially on white stones. Concerning the reduction of protective efficacy, the lone pair of electrons on the oxygen atoms, are deactivated by the fluorine atoms present in the molecule, so they are not available for the interaction between this polymer and the stone surface. Due to the very weak interactions the perfluopolyethers on the surface they slowly tend to migrate inside the stone, that is they are absorbed by the porous structure. The mobility of the product inside the stone leads to a gradual loss of the coating on the surface in the course of time, reducing its efficacy. On some lithotypes, (e.g. sandstones) this inward diffusion is sufficiently slow due to the texture of calcium carbonate and the presence of clay layers,
ensuring a protective efficacy for a long time, while in many other cases (e.g. marble or tiles) this phenomena causes a rapid decrease of the surface protection and requires further treatments in the course of time.
Scheme 6. Synthesis of some important families of perfluoropolyethers with commercial names.
In order to reduce the mobility of perfluoropolyethers, some new products were prepared, containing polar groups able to form chemical or physical interactions with the substrate. Perfluoropolyetheric carboxylic acids, esters and amides were very interesting
products due to the possibility to transform their functional group in compounds having the possibility to interact with the stone support [30, 35, 36].
Perfluoropolyetheric amides were obtained as viscous liquid having high chemical stability. Their properties made them eligible as protective agents for stone objects of relevant historical and artistic importance, in particular for those exposed to an aggressive environment. The use of these functionalized perfluoropolyethers gave very good results in the protection of marble and other stones having low or medium porosity and quite good results were also obtained with high porosity materials.
On the other hand, the application of these compounds required the use of chlorofluorocarbons as solvents. In the Nineties, the Montreal international protocol declared the CFC very dangerous for the environment and they were blamed as the main cause of the formation of the ozone hole. The use of these solvents was gradually banned, making the application of perfluoropolyethers very hard. In the literature it was proposed to bypass this problem using aqueous micro-emulsion of perfluoropolyether derivatives, but this application is not easily performed . It is also known the use of dispersion or aqueous emulsions of fluorinated polyurethanes for treating marble stones, bricks and similar materials used in buildings and historical monuments . They were obtained by polymerization of perfluoropolyethers having hydroxyl terminal groups with di-isocyanates.
Many other examples of fluorine containing polymers have been reported in the literature. Among these, partially fluorinated acrylic and methacrylic polymers are particularly interesting, considering their suitable Tg, solubility in many organic solvents, water repellence, adhesive and cohesive properties [39-41]. These polymers may be subdivided into polymers containing fluorine in the ester group or polymers containing fluorine in the main chain (Figure 2). Usually, acrylic and methacylic monomers
containing fluorine atoms in the ester group are commercially available, while monomers containing fluorine atoms in the main chain must be synthesised in laboratory through complex procedures.
Acrylates containing fluorine atoms in the ester moiety are obtained by partial or total replacement of the methacrylate units in Paraloid-B72 (EMA/MA) with fluorinated methacrylates. The expected improvement of the coating properties was not reached: although side chain fluorination of acrylic copolymers usually improves the hydrophobicity of the polymer, in this case the photostability was only slightly improved. Presumably the fluorine atoms were too far from the weak tertiary C–H bonds to provide a significant stabilization effect. Furthermore in the course of the ageing the ester moiety containing fluorine atoms were rapidly lost.
Polyacrylates containing fluorine atoms in the main chain, such as poly(ethyl 2-fluoroacrylate) (PE2FA), showed a stabilizing effect of the fluorine atom on the rate of oxidation. Among the different partially fluorinated acrylic and methacrylic polymers, PE2FA showed the highest chemical stability and it was proposed as protective agents for stone [42, 43]. Copolymers between a methacrylic ester and a modified perfluoropolyether has been obtained by insertion of a perfluoropolyetheric moiety in the course of the polymerization. This process may be performed by Atom Transfer Radical Polymerization (ATRP), using a functionalized perfluoropolyether as radical initiator of the reaction .
Figure 2. Some examples of fluorinated acrylates and methacrylates.
In recent years a new class of fluorinated polymers, produced from natural and renewable sources, has been developed and its importance is rapidly growing among conservation materials. These new materials share the basic chemical structure of polylactic acid.
Polylactic acid (PLA) has attracted considerable attention in the last decades due to its synthesis from renewable resources, controlled polymerization, good mechanical properties, processability and inherent biocompatibility . PLA advantages over conventional petroleum-based plastics include: (1) production of the lactide monomer by fermentation of renewable agricultural feedstocks (corn) instead of gas and oil resources, (2) fixation of significant quantities of carbon dioxide by plants for corn production, (3) significant oil saving in the production process, (4) easiness of recycling back to lactide and lactic acid by hydrolysis or alcoholysis with formation of byproducts having a low toxicity, (5) biodegradability, (6) ability to tailor physical and mechanical properties through controlled synthesis and post-modifications .
The starting material for the production of PLA, that is lactic acid, can be produced from many natural sources (corn, sugar beet, or other sugar containing materials), by a fermentation process. Oligomers of lactic acid are produced by polycondensation or azeotropic distillation. In order to obtain high molecular weight polymers, useful for industrial applications, a Ring Opening Polymerization (ROP) process is performed (Scheme 7), catalyzed by Sn(II) Octoate, (Sn(II)-2-ethylhexanoate) (SnOct2). The monomer of the ROP process is lactide (3,6-dimethyl-1,4-dioxane-2,5-dione), obtained by high temperature depolymerization (back-biting reaction) of lactic acid oligomers produced by polycondensation .
PLA can reach a maximum value of Tg = 60 °C, and Tm = 180 °C, it is biodegradable, it is not harmful for man and environment and it is approved by Federal Drug Administration.
Scheme 7. Mechanism of the ROP process of lactide.
FUNCTIONALIZATION OF POLYLACTIC ACID
Functionalization of polylactic acid and polylactides in general address two critical issues in polymer science: degradability and utility. The ability of tuning the physicochemical properties of the polymer (hydrophobicity, degradability, thermal properties, etc.) is a key point for obtaining materials suited to specific applications (tailor made materials). Three strategies have been developed to introduce functionalities into the polylactide scaffold: the traditional (TD) approach, the functional monomer (FM) approach and the post-polymerization modification (PPM) approach (Scheme 8). These routes incorporate functional groups onto the polymer backbone to enhance properties or act as access points for further modification.
Scheme 8. Different routes to PLA functionalization (FG = functional group).
In the following paragraphs the functional monomer approach will be treated in details, since it is the procedure adopted in this research.
Functional monomer route
Lactide monomer is obtained by depolymerization of lactic acid oligomers, that in turn are obtained by fermentation of sugar extracted from corn plants. Since only a few other α-hydroxy acids can be isolated by fermentation, such as 2-hydroxyisocaproic acid  and β-phenyllactic acid , most functionalized monomers rely on the synthesis of unique starting materials. As shown in Scheme 9, there are two general synthetic routes to prepare functionalized glycolide monomers: (1) symmetric glycolides are prepared by synthesizing functionalized α-hydroxy acids, which are dimerized in dilute organic
solvents , and (2) asymmetric AB glycolides are prepared by a two-step condensation between an α-hydroxy acid and a 2-halo-alkanoyl halogenide via an α-haloester intermediate, as firstly reported by Schollkopf et al .
Scheme 9. General scheme of the synthesis of symmetric and asymmetric glycolides.
Alkyl-substituted polyglycolides have been synthesized by polymerization of cyclic dimers derived from the corresponding α-hydroxy acids, which in turn are obtained by enzymatic α-hydroxylation of fatty acids or by standard synthetic methods. Most
standard syntheses follow one of two routes (Scheme 9): reaction of Grignard reagents with diethyl oxalate, followed by reduction and hydrolysis of the α-ketoester, or hydrolysis of the cyanohydrin formed upon reaction of potassium cyanide with the corresponding aldehyde. Using these methods, polyglycolides with n-alkyl chains up to 16 carbon atoms have been prepared . Increasing the steric bulk of the substituents attached to the polymer backbone should increase the Tg, as reported for polyolefins. However differential scanning calorimetry (DSC) of polyglycolides showed the opposite trend: longer alkyl chains decreased the Tg. This behavior was probably due to the linear alkyl chains that decreased dipole-dipole interactions between the ester groups in the polymer backbone.
If linear chains decrease the Tg, then branched alkyl chains would more effectively increase the Tg. Although several polyglycolides with branched chains have been synthesized, there were only minor structural diversities on polymer properties . For example in poly(isopropylglycolide), a lactide analogue of polyvaline, the isopropyl group is directly attached to the polymer backbone, while in poly(isobutylglycolide) the isopropyl group is placed one carbon from the polymer chain. The Tg of poly(isopropylglycolide) and poly(isobutylglycolide) are respectively 50 °C and 23 °C, demonstrating the importance of placing the bulky group adjacent to the polymer backbone. The isopropyl group is more sterically demanding than the methyl group of lactide but the Tg was not significantly increased, thus dipole-dipole interactions were not effectively screened. A significant increase in the Tg was showed by poly(cyclohexylglycolide), with a Tg of 98 °C . The steric hindrance caused by cyclohexyl groups was sufficient to hinder rotation of the polymer backbone and increase the Tg.
Scheme 10. Comparison between copolymerization of symmetric glycolides and homopolymerization of asymmetric glycolides.
Asymmetric monomers provide another route to structural diversity in polyglycolide polymers. Polymerization of AB monomers, where two different glycolic acid derivatives are incorporated into one glycolide ring, is analogous to copolymerization (Scheme 10). However, while copolymerization gives a random copolymer, polymerization of asymmetrical monomers in principle gives a perfectly alternating copolymer. The growing chain end in an AB system discriminates between two different sites on the same glycolide monomer rather than between two comonomers. For glycolides with simple alkyl and aryl substituents, steric effects largely define the rate of ring opening polymerization and increasing the difference in the relative sizes of the two ring substituents favors alternation. Figure 3 shows some examples of alkyl-substitued polyglycolides and their Tg, prepared from symmetric and asymmetric monomers by Baker et al. [52-55] and Trimaille at al. .
Figure 3. Alkyl-substituted polyglycolides with their respective Tg.
Aryl-substituted polyglycolides are promising candidates for high Tg polymers by analogy with polyolefins. For example, while atactic polypropylene has a Tg of -11 °C, polystyrene has a Tg of 109 °C. One of the simplest starting materials for the synthesis of
polylactides analogous to polystyrene is phenyllactide, made available by various biosynthetic pathways . Polymers based on phenyllactide and its derivatives were synthesized and studied [56, 58]. Poly(phenyllactide) seemed the perfect candidate for high Tg polymers, considering the presence of a bulky aromatic ring and the possibility of π-π interactions, however the Tg of high molecular weight polymer was only 50 °C. Although the Tg was comparable to that of poly(isopropylglycolide), it is significantly higher than poly(isobutylglycolide), containing a methylene group between the bulky group and the polymer backbone. As expected, the steric effects of aromatic rings, as well as alkyl groups, decrease as they are moved farther from the polymer backbone. To further increase the steric bulk, methyl groups were added to the aromatic rings. (4-methylphenyl)lactide was synthesized and polymerized to high molecular weight, increasing the Tg to 59 °C, an improvement over poly(phenyllactide), but still too low for a high Tg material. The meta and ortho derivatives were also investigated and are suspected to have greater effects on increasing the Tg due to higher steric demands, however, their syntheses were problematic, and no reliable Tg data were reported.
Comparing the Tg of polystyrene and poly(allylbenzene), a structural analogue of poly(phenyllactide), suggests that using methylene groups to link the aromatic rings to the polymer backbone causes a 30 °C drop in Tg. Using this logic, direct attachment of the aromatic ring to the polyglycolide backbone should significantly increase Tg. Thus, mandelide, the cyclic dimer of mandelic acid should provide the appropriate structure. Like lactic acid, mandelic acid is a naturally occurring metabolite and in principle, poly(mandelide) synthesis could be a bio-based process. Early attempts to synthesize poly(mandelide) were hindered by impurities in the monomer employed that acted as initiators and limited the molecular weight. The synthesis of poly(mandelide) presented several challenges, most notably racemization and reduced monomer solubility, however,
Liu et al. was able to produce high molecular weight polymers with Tg of 100 °C . The materials were colorless, glassy amorphous solids, similar to polystyrene. The rate of hydrolysis and biodegradation of the materials with respect of poly(lactide) were several times lower due to the increased hydrophobicity caused by the presence of phenyl rings. However, poly(mandelide) may not be a perfect substitute of polystyrene due to yellowing developed during melt processing of the polymer, most likely a result of the highly reactive methine protons which are in α position to both a carbonyl and a benzene ring.
Figure 4 shows some examples of aryl-substitued polyglycolides and their respective Tgs.
The synthesis of hydroxy-functionalized polyglycolides present an intrinsic challenge: the presence of the alcohol group in the polymer structure. Water and alcohols are well known initiators in the polymerization of lactide and lactone monomers, therefore the alcohol groups must either be introduced by post-polymerization reactions or via a protection/deprotection pathway. Feng and co-workers firstly introduced hydroxy-functionalized glycolide, 3-benzyloxymethyl-1,4-dioxane-2,5-dione (3-BMG), starting from 3-chloropropanediol (Scheme 11) . Ring opening polymerization (ROP) catalyzed by Sn(ll)-2-ethylhexanoate (SnOct2) generated an amorphous polymer with a Tg of 34 °C. Deprotection via catalytic hydrogenation removed the pendant benzyl groups, resulting in a water-soluble polymer, poly(3-hydroxymethyl-1,4-dioxane-2,5-dione) (poly(3-HMG)). The contact angle and the Tg of the polymer decreased upon deprotection.
A more versatile route to hydroxy-lactide monomers was reported by Gerhardt et al.  and later by Leemhuis et al. (Scheme 12) . They obtained optically pure hydroxyl glycolides from optically pure O-Bn-L-serine starting material. In the synthesis of lactide derivatives however, rac-2-bromopropionyl bromide was used in the intramolecular ring closing reaction and two diastereomers were formed. The two diastereomers were separated by flash column chromatography and the (S,S) isomer was used for polymerizations. Leemhuis also compared the polymerization rates of the lactide- and glycolide-substitued benzyloxymethyl monomers, using ethylzinc phenolate and 2-propanol as the catalyst and initiator, respectively. Crystal structure analysis revealed that the OBn and methyl substituent in OBn-L-Ser-LD monomer are both in equatorial positions of the dilactone ring. Since the groups presented almost identical steric demands, both carbonyls were nearly equally accessible and polymerization yielded a random polymer. However in OBn-L-Ser-GLY, replacement of the methyl group with hydrogen results in a clear structural difference and preferential opening at the less hindered carbonyl, creating an alternating polymer. DSC analysis showed that both polymers were completely amorphous with Tg of 30 °C and 25 °C for poly(OBn-L-Ser-LD) and poly(OBn-L-Ser-GLY), respectively. The protecting groups were removed from the two polymers via catalytic hydrogenation using Pd/C (10 %) and THF as a solvent. The homopolymers were completely deprotected after 24 hours and GPC showed no chain scission. Deprotected poly(L-Ser-LD) was completely amorphous with a Tg of 30 °C, while poly(L-Ser-alt-Gly) was semi-crystalline with a Tg of -4 °C and a Tm of 135 °C. Polymer was not soluble in aqueous solution . Gerhardt and co-workers obtained a poly(QBn-L-Ser-GLY) with molecular weight of 21 kD by ROP, using SnOct2 as the catalyst. The amorphous polymer had a Tg of 18 °C and was deprotected by
hydrogenolysis using Pd(OH)2; however molecular weight and Tg for the deprotected polymers were not reported .
Scheme 12. Synthesis, polymerization, and deprotection of Ser-GLY and OBn-L-Ser-LD.
A different approach to hydroxy-functionalized glycolides was described by Marcincinova et al. In their syntheses of 3-(1,2,3,4-tetraoxobutyl-diisopropylidene)-dioxane-2,5-dione (DiPAGYL) and 3-methyl-6-(1,2,3,4-tetraoxobutyl-diisopropylidene)-dioxane-2,5-dione (DiPALAC), monomers was composed by a glycolyl and a D-gluconyl unit derived from gluconic acid (Scheme 13) . After selective protection of the four pendant hydroxy groups with 2,2-dimethoxypropane and intramolecular ring closure with
bromoacetyl chloride or 2-bromopropionyl chloride, monomers were isolated as white crystals. Ring opening polymerization of DiPAGYL led to a 20 kD brittle amorphous polymer with a Tg of 95 °C. All attempts to polymerize DiPALAC led to oligomers with molecular weights of ≈ 2 kD. Several methods to remove the isopropylidene groups were investigated, all under acidic conditions, but degradation of the polyester backbone was always obtained . The best results were accomplished using iodine in methanol or aqueous acetic acid; however even these methods showed modest degradation, with the maximum deprotection of 60 %, as determined by NMR. At 60 % deprotection, a fully protected 32 kD polymer degraded to 5 kD (versus 27 kD theoretical value). The partially deprotected polymers were soluble in hydrophilic solvents such as methanol and ethanol and were partially soluble in water.
Scheme 13. Synthesis, polymerization, and partial deprotection of DiPAGYL and DiPALAC.
Carboxylic acid-substitued polyglycolides
The introduction of hydrophilic groups, such as carboxylic acids, in the polylactide backbone is important for biomedical and pharmaceutical applications. Since the hydrolysis rates of poly(α-hydroxyacids) are often low and limited by crystallinity. Methods to decrease crystallinity and hydrophobicity are important for in vivo applications, some of which require water soluble polymers.
Scheme 14. Synthesis, polymerization, and deprotection of 3(S)-[(benzyloxycarbonyl)methyl]-1,4-dioxane-2,5-dione.
The synthesis of 3(S)-[(benzyloxycarbonyl)methyl]-1,4-dioxane-2,5-dione is described by Kimura and co-workers . The polymerization yielded an alternating copolymer consisting of glycolic acid and benzyl α-(S)-malate units (Scheme 14). Ring-opening polymerizations were run in solution or bulk, utilizing SnOct2 or Et2Zn (diethyl zinc) as the catalyst. Molecular weights ranged from 2 kD to 21 kD. The polymers were deprotected via catalytic hydrogenolysis using platinum oxide or palladium on carbon yielding crystalline, water-soluble polymers. Molecular weights were not reported for the deprotected polymers. The copolymerization with lactide yielded a random copolymer
that hydrolized more rapidly than polylactide thanks to the hydrophilic pendant carbonyl units .
L-malic acid (L-MA) or L-aspartic acid (L-AA) were used to prepare malide dibenzyl ester, the cyclic dimer of β-benzyl malate, by Ouchi and co-workers . The best yields were obtained using L-MA (Scheme 15). Ring-opening polymerization was carried out at 220 °C using organotin compounds as catalysts. The protecting groups were removed by hydrogenation using palladium on carbon and EtOAc as solvent.
Scheme 15. Synthesis of malide dibenzyl ester from L-malic acid (L-MA) or L-aspartic acid (L-Asp), polymerization, and deprotection.